Civil and Environmental Research ISSN 2224-5790 (Paper) ISSN 2225-0514 (Online) Vol.3, No.4, 2013
studied. Figure 6 shows that the longer the coconut fibers and the lower the coconut fiber content, the lower the ductility values were.
Figure 6. Relationship between CFA content and softening point 3.4. Moisture susceptibility The adverse effect of moisture on the resistance of asphalt mixtures is expressed by the strength ratio (SR). The SR is defined as the ratio of dry and wet strength specimens. The higher the SR, the better the resistance to moisture damage of the asphalt mixtures. Most pavement agencies recommend that the SR value be greater than 70-80% in their mixture design specifications (Roberts et al, 1996). As shown in Table 5, the SR values obtained for both mixtures are greater than 80%, which meets the mixture design specifications. However, the SR of the CFA-modified (94%) is approximately 2% lower than that of the conventional mixture (96%). An SR value of 94% indicates that negligible moisture damage has occurred in the modified CFA wet specimens. This resistance, which meets the minimum requirements of the modified CFA to moisture damage, could be mainly attributed to the anti-stripping agent. Figure 7 shows the Marshall stability of dry and wet samples with different contents of coconut fiber. Table 5 Moisture susceptibility results Coconut fiber content (%) 0 0.5 0.75 1 1.25 1.5
Dry Air void (%) 3.49 4.14 3.01 3.52 4.19 4.57
Air void (%)
1,008.7 1,070.3 1,332.2 1,209.0 1,147.3 1,093.4
3.74 4.45 3.43 3.99 4.94 5.42
970.2 1,016.4 1,216.7 1,124.2 1,062.6 1,039.5
Strength ratio (%) 0.96 0.95 0.91 0.93 0.93 0.95
The desirable properties of asphalt mixtures for flexible pavement surfacing are stability, durability, flexibility, and skid resistance (Jitsangiam et al, 2013). Conventional hot mix asphalt (HMA) design methods aim to determine the optimum asphalt content at which the asphalt layer performs satisfactorily, particularly with respect to stability and durability (Asi et al, 2007).